Corrosion inhibition efficiencies of some common reported organic and chitosan based corrosion inhibitors in aggressive solution.
Development of non-toxic and environmental friendly corrosion inhibitors is highly desirable owing to the increasing demands of “green chemistry” throughout the world. In view of these several forms of green corrosion inhibitors such as drugs or medicines, plant extracts, ionic liquids and synthetic inhibitors derived from multicomponent reactions (MCRs) and mechanochemical mixing are being employed. Nowadays, MCRs in association with microwave and ultrasound irradiations represent one of the best green strategies. Natural polysaccharides particularly chitosan derivatives gained substantial advancement. Chitosan and its several derivatives have been employed effective as corrosion inhibitors for metals and alloys in various aggressive media. The present chapter features the collection of major works that have been published on the inhibition effect of chitosan and its derivatives. The utilization of the chitosan and its derivatives as effective corrosion inhibitors is based on the fact that they contain several polar functional groups such as amino (-NH2), hydroxyl (-OH) and acetyl (-COCH3) groups that effectively bind with metallic surface and behave as adsorption centers.
- green corrosion inhibitors
- aggressive solution
- mixed-type inhibitors
Alloys steel such as carbon steel and mild steel have been extensively utilized as construction materials for several purposes because of their high mechanical strength and cost-effective behaviors. However, they are highly reactive and undergo corrosion when exposed to the environment particularly in acid treatment processes like acid cleaning, acid descaling, acid pickling and oil well acidification. Therefore, these cleaning processes require application of some external additive to avoid the corrosive dissolution of metallic materials. The external added chemical species are known as corrosion inhibitors. It is important to mention that the difference in the mild steel and carbon steel is the amount of carbon. Mild steel has relatively small amount of carbon ranging from 0.16 to 0.30%. Carbon steel contains larger amount of carbon, generally ranging from 0.30% to more than 2% [1, 2]. Among several available methods of corrosion protection, the utilization of organic compounds is one of the most appropriate and cost-effective methods. The extensive utilization of the organic compounds as corrosion inhibitors is also attributed due to their high effectiveness and ease of application. These compounds adsorb and form a corrosion protective barrier by transferring their non-bonding and π-electrons into the metallic d-orbitals. The electron transferring (Adsorption) ability of these compounds influences by several factors such as electronic structure of the compound, nature of metal and corrosive environment, surrounding temperature, presence of impurities, exposure duration etc. [3, 4]. The polar functional groups of heteroatoms (N, O, and S) such as –CN, -OH, -NH2, -OCH3, -COOH, -CONH2, -COOC2H5 etc. and double and triple bonds behave as adsorption centers [3, 4]. It is reported that these polar functional groups easily undergo protonation in strong acidic medium like 1 M HCl and exist in their cationic form. On the other hands, metallic surface becomes negatively charge due to the adsorption of counter ions of electrolyte (chloride ion in HCl). These two oppositively charged species attracted each other through electrostatic force of attraction (physisorption mechanism). In the later stage of the adsorption phenomenon neutral heteroatoms transfer their unshared electron pairs to the empty d-orbitals of the surface metallic atoms to form coordinate bonds that results in to the chemical adsorption. Recently, the growing natural awareness and severe environmental guidelines demand application of the compounds for different purposes that have been originated from natural and biological resources. The chemical synthesis of the organic compounds is not only expensive but also causes discharge of several toxic chemicals into the surrounding environment that can have several adverse effects on living beings. The increasing demands of “green and sustainable chemistry” throughout the world, forces to the scientists working in the field of corrosion chemistry to grow highly desirable “green and sustainable corrosion inhibitors” either by deriving them from natural resources or by synthesizing them using suitably modifying the available synthetic methods. In last two decades, use of multicomponent reactions (MCRs), chemical reactions catalyzed by energy efficient microwave and ultrasound irradiations, plant extracts, chemical medicines (drugs), ionic liquids etc. toward “green and sustainable corrosion inhibition” have gained significant milestone in this direction.
In recent decades, the use of carbohydrates and their derivatives as metallic corrosion inhibitors has been a growing effort to decrease the environmental pollution [3, 4]. Natural availability, biosynthesis using greenhouse (CO2) gas, biodegradability, biocompatibility, and high solubility in aqueous media make the carbohydrates as “green” chemicals for variety of chemical transformations [5, 6, 7]. The carbohydrates act as inhibitor for protein glycosylation activities, medicines for bacterial infections (antibiotics), viral infections (antiviral), neuronal proliferation, cancer metastasis and apoptosis [8, 9, 10]. Additionally, carbohydrate derivatives (including chitosan) are extensively used as detergent, food, and cosmetics, sweetening agents, cloths, paper, lumber and other variety of other purposes [10, 11, 12]. Chitosan is polymeric form of deacetylated chitin with a variety of properties such as immunological activities, low toxicity, wound healing and biodegradability [13, 14]. The chemical structure of chitosan is shown is shown in Figure 1.
Similar to most of the carbohydrates, chitosan is rich in functional groups (hydroxyl and amino) it would be a potential inhibitor for metallic corrosion [15, 16]. The amount of amino group in chitosan is determines by degree of deacetylation. Chitosan and its derivatives are important materials having several industrial and biological applications. These materials are gaining attention in food, biomedical, agricultural, environmental and pharmaceutical industries because of their non-toxic, environmental-friendly, non-allergenic and biocompatible nature. Their diverse biological applications include anti-hypertensive, anti-oxidant, anti-diabetic, anti-coagulant, anti-inflammatory, anti-microbial, anti-obesity, anti-cancer and neuro-protective properties [17, 18]. The hydroxyl (-OH) group at 6-position and amino (-NH2) group at 2-position are the most chemically reactive sites of chitosan for modification procedures. Chitin is natural source of chitosan which is mainly distributed in the shells of crabs and shrimp, in the cell of fungi and cuticles of insects [13, 14]. The chitosan can be derived by N-deacetylation of chitosan using several deacetylation agents. The chitosan and its derivatives are being utilized for variety of purposes because of their biocompatibility, non-toxic nature, high biodegradability, high 1 wound healing behavior and immunological activity, etc. [19, 20, 21, 22, 23].
2. Main body
Because of their green and environmental friendly nature chitosan and its derivatives are being utilized as effective corrosion inhibitors for metals and alloys for several electrolytic media including HCl, H2SO4 and NaCl etc. The corrosion inhibition property of chitosan and its derivatives in correlation with other commonly employed organic and inorganic corrosion inhibitors are presented in Table 1. Abd-El-Nabey et al.  demonstrated the inhibition properties of chitosan in 0.1 M HCl using potentiodynamic polarization (PDP) and electrochemical impedance spectroscopic (EIS) methods. Chitosan showed the optimum inhibition efficiency of 90% at 0.028 g/L concentration. EIS study revealed that chitosan adsorbs at metal/ HCl interface and behaved as interface corrosion inhibitors. PDP study showed that chitosan behaved as mixed type corrosion inhibitor.
|Type of inhibitors||Name of inhibitor||Nature of metal and electrolyte||Adsorption behavior||Highest efficiency and concentration||Ref.|
|Organic inhibitors||2, 2′-bis(benzimidazole)||Mild steel/1 M HCl||Mixed type/Langmuir adsorption isotherm||97.8% at 10−4 M|||
|2, 5-bis (4-methoxyphenyl)-1,3,4-oxadiazole||Mild steel/1 M HCl||Mixed type/Langmuir adsorption isotherm||96.19% at × 10−4 M|||
|Pyridine-2-thiol (P2T) and 2- Pyridyl disulfide (2PD)||Mild steel/in flow HCl||Mixed type/Langmuir adsorption isotherm||More than 98% 200 mg/L|||
|4,4-dimethyloxazolidine-2-thione (DMT)||Mild steel/1 M HCl||Mixed type/Langmuir adsorption isotherm||82% at 4 × 10−3 M|||
|2-mercapto benzimidazole (2MBI)||Mild steel/1 M HCl||Mixed type/ Langmuir adsorption isotherm||98% at 10−3 M|||
bromide and N-octadecylpyridinium bromide
|Mild steel/1 M H2SO4||Mixed type/Langmuir adsorption isotherm||82% and & 88% at 100 ppm|||
|Tryptamine||Mild steel/0.5 M H2SO4||Mixed type/Langmuir adsorption isotherm||97% at 500 ppm|||
|N-Phenyl oxalic dihydrazide (POD-H) and oxalic N-phenylhydr-azide N′- phenylthiosemicarbazide (OPHPT)||Mild steel/1 M HCl||Mixed type/Langmuir adsorption isotherm||92% for OPH-PT and 79% for PODH|||
|Cysteine||Copper/1 M HCl||Cathodic type/Langmuir adsorption isotherm||84.13% at 18 mM|||
|Chitosan based inhibitors||Chitosan||Al, Mild steel/ 0.1 M HCl||Mixed type||More than 90% at 0.028||[24, 34]|
The inhibition property of the chitosan on mild steel corrosion in 0.1 M HCl has also been investigated using gravimetric, PDP, EIS, scanning electron microscopy SEM and UV-visible methods . At 60°C temperature chitosan showed 96% inhibition efficiency which drops to 93% on increasing temperature 70°C . Chitosan acted as mixed type corrosion inhibitors as observed by PDP study. Adsorption of the chitosan on mild steel surface obeyed the Langmuir adsorption isotherm. EIS study showed the chitosan acted as interface corrosion inhibitor that is retards the corrosion process by adsorbing on the metal/ electrolyte interface [35, 36, 37]. The inhibition property of chitosan for corrosion of copper in 0.5 M HCl has also been studied weight loss, PDP, EIS and electrochemical frequency modulation (EFM) measurements . Chitosan acts as mixed type inhibitor and its adsorption obeyed the Langmuir adsorption isotherm. The high protection ability of the chitosan forced the people working in the field of corrosion to develop and use of chitosan derivatives as corrosion inhibitors. Cheng and his coworkers  demonstrated the inhibition property of carboxymenthylchitosan (CM-chitosan) as ecofriendly corrosion inhibitors for mild steel in 1 M HCl using weight loss, EIS and PDP techniques. The structure of CM-chitosan is shown in Figure 2.
The CM-chitosan showed maximum protection ability of 93% at 200 mg/L concentration. Adsorption of the CM-chitosan on mild steel surface obeyed Langmuir adsorption isotherm. PDP study suggested that CM-chitosan acted as mixed type corrosion inhibitor. In other study , these authors studied the effect of cupric (Cu2+) ions on corrosion inhibition property of CM-chitosan toward acidic dissolution of mild steel in 1 M HCl. Results showed that CM-chitosan+Cu2+ showed better protection ability much more effectively than the inhibiting action of each additive separately. In continuation of this type of works, acetyl thiourea chitosan polymer (ATUCS) was synthesized and investigated as effective inhibitor for mild steel in aerated 0.5 M H2SO4 solution using EIS, PDP and SEM methods . The chemical synthesis of ATUCS is shown in Figure 3.
Results showed that ATUCS acted as interface corrosion inhibitor and its adsorption on mild steel surface obeyed the Langmuir adsorption isotherm. The ATUCS acted as mixed type corrosion inhibitor. Two formaldehyde based chitosan derivatives based on thiosemicarbazide (TSFCS) and thiocarbohydrazide (TCFCS) (Figure 4) were synthesized and investigated as effective corrosion inhibitors for heavy metals . TCFCS behaved as mixed type corrosion inhibitor and showed maximum efficiency of 92% at 60 mg/L concentration.
The new compounds were characterized and studied by Fourier transform infrared spectroscopy, elemental analysis, thermal gravity analysis and differential scanning calorimetry, and their surface morphologies were determined via scanning electron microscopy. The inhibition effect of two chitosan derivatives namely 2-N,N-diethylbenzene ammonium chloride N-oxoethyl chitosan (compound I), and 12-ammonium chloride N-oxododecan chitosan (compound II) on carbon steel corrosion in 1 M HCl using weigh loss method has been reported . Along with the antibacterial property these compounds showed good corrosion inhibition efficiency toward carbon steel corrosion in acidic medium. The authors claimed that functionalization of the chitosan into compound I and II causes significant change in the physiochemical properties. The enhanced solubility in the polar testing solution (1 M HCl) due to presence of polar amino (-NH2) and several hydroxyl (-OH) groups the functionalized chitosan molecules adsorb efficiently on the metallic surface and showed good corrosion inhibition efficiency. These compounds inhibit corrosion by adsorption mechanism and their adsorption of compound I and compound II obeyed the Langmuir adsorption isotherm. Compound I showed highest inhibition efficiency among the tested compounds. These authors also observed that the antibacterial activity of chitosan for Enterococcus faecalis,
|Inhibitors||Inhibitor Conc. (mg L−1)||Surface coverage (θ)|
Besides the use of chitosan and its derivatives as solution phase corrosion inhibitors, few organic and inorganic composites of chitosan have also been used as coating materials for protection of their dissolution in aggressive environments. Pang and Zhitomirsky  coated 316 L stainless steel hydroxyapatite-chitosan and characterized them using X-ray diffraction (XRD), thermo-gravimetric and differential thermal analysis, scanning and transmission electron microscopy, PDP and EIS methods. Electrochemical investigations showed that the obtained coatings provide the corrosion protection of the 316L stainless steel substrates. The heat treatment of the coating at 140°C resulted in an improved corrosion protection. The crotonaldehyde based chitosan Schiff’s base derivative designated as Ch-Cr-SB (Figure 5) was synthesized and coated on the surface of AZ91E alloy for its anticorrosive behavior .
The protection abilities of chitosan and chitosan derived SB was compared in the present study. The electrochemical corrosion behavior has been also studied for Ch-Cr-SB in aerated 3% NaCl solution containing different concentrations of Schiff’s base, in the range from 0.03 to 0.075 mM, using different. Results showed that presence of these inhibitors in the corrosive 3% NaCl solution decreases the rate of corrosion. The chitosan electrochemically deposited over the metallic surface from the solution of chitosan in acetic acid. In order to further improve the effectiveness of coating, coated samples were further treated with formaldehyde solution. The coating of chitosan on mild steel surface was measured by FTIR, SEM, PDP and EIS methods . The coating samples showed improvement in the protection ability up to 98.1% at 0.5 M H2SO4. A significant increase in the charge transfer resistance was observed for coated mild steel surfaces. The electro-deposition of Zn-chitosan composite coating on mild steel and its corrosion studies has been reported in 3.5% NaCl , Self-healing protective coatings with chitosan based pre-layer reservoir , chitosan/diclofenac coatings for medical grade stainless steel , copper modified chitosan inhibition of AA-2024 corrosion , 2-Mercaptobenzothiazole (MBT) based functionalized chitosan-based coatings for active corrosion protection of AA2024 alloy , chitosan/Silver nanoparticles composite on St37 steel corrosion in a 15% HCl solution , self-healing protective coatings chitosan doped with cerium nitrate for inhibition of aluminum alloy 2024  and Poly(itaconic acid)-modified chitosan for inhibition of aluminum corrosion  and other composites materials have also been investigated as effective chitosan based coatings.
Chitosan and its derivatives are important class of natural/bio-polymers that have several biological and industrial applications. They are used as anti-oxidant, anti-hypertensive, anti-inflammatory, anti- diabetic, anti-coagulant, anti-obesity, anti-microbial, anti-cancer and neuro-protective agents. Their extensive use and demands based on the facts that these compounds are non-toxic, environmental-friendly, biocompatible, commercially availability and non-allergenic behavior. In view of the above it is concluded that chitosan and its derivatives are “green and sustainable materials” to be used for their various applications. Present chapter deals with the collections of reports available on the corrosion inhibition properties of chitosan and its various derivatives. The ongoing discussion showed that chitosan based compounds represent a green and sustainable class of corrosion inhibitors and can be successfully employed at the place of traditional toxic corrosion inhibitors. These inhibitors can be derived either from biological systems or can be synthesized in laboratories from the hydrolysis of chitin and further functionalization. Chitosan and its derivatives act as efficient solution phase inhibitors for mild steel, carbon steel, copper and aluminum. Generally, there adsorption on metallic surface obeyed the Langmuir adsorption isotherm. PDP study revealed that chitosan and its derivatives behaved as mixed type corrosion inhibitors. Through electrochemical impedance spectroscopic measurement it can be derived that chitosan and its derivatives behaved as interface type of corrosion inhibitors that is they adsorb at the interface of metal and electrolytic solution. Chitosan and its derivatives have also been used in coating for protection of metallic and alloys dissolution in aggressive media like NaCl and HCl solution.
Higuchi M, Iida K. Fatigue strength correction factors for carbon and low-alloy steels in oxygen-containing high-temperature water. Nuclear Engineering and Design. 1991; 129:293-306
Grange R, Baughman R. Hardness of tempered martensite in carbon and low alloy steels. Transactions of American Society for Metals. 1956; 48:165-197
Verma C, Olasunkanmi LO, Ebenso EE, Quraishi M, Obot I. Adsorption behavior of glucosamine-based, pyrimidine-fused heterocycles as green corrosion inhibitors for mild steel: Experimental and theoretical studies. The Journal of Physical Chemistry C. 2016; 120:11598-11611
Verma C, Quraishi M, Kluza K, Makowska-Janusik M, Olasunkanmi LO, Ebenso EE. Corrosion inhibition of mild steel in 1M HCl by D-glucose derivatives of dihydropyrido [2, 3-d: 6, 5-d′] dipyrimidine-2, 4, 6, 8 (1H, 3H, 5H, 7H)-tetraone. Scientific Reports. 2017; 7
Kobayashi Y, Suzuki M, Satsu H, Arai S, Hara Y, Suzuki K, Miyamoto Y, Shimizu M. Green tea polyphenols inhibit the sodium-dependent glucose transporter of intestinal epithelial cells by a competitive mechanism. Journal of Agricultural and Food Chemistry. 2000; 48:5618-5623
Kobayashi H, Fukuoka A. Synthesis and utilisation of sugar compounds derived from lignocellulosic biomass. Green Chemistry. 2013; 15:1740-1763
Daoutidis P, Kelloway A, Marvin WA, Rangarajan S, Torres AI. Process systems engineering for biorefineries: New research vistas. Current Opinion in Chemical Engineering. 2013; 2:442-447
Farrán A, Cai C, Sandoval M, Xu Y, Liu J, Hernáiz MJ, Linhardt RJ. Green solvents in carbohydrate chemistry: From raw materials to fine chemicals. Chemical Reviews. 2015; 115:6811-6853
Laurienzo P. Marine polysaccharides in pharmaceutical applications: An overview. Marine Drugs. 2010; 8:2435-2465
Gupta S, Abu-Ghannam N. Bioactive potential and possible health effects of edible brown seaweeds. Trends in Food Science & Technology. 2011; 22:315-326
Thomas NV, Kim S-K. Beneficial effects of marine algal compounds in cosmeceuticals. Marine Drugs. 2013; 11:146-164
Chatterjee C, Pong F, Sen A. Chemical conversion pathways for carbohydrates. Green Chemistry. 2015; 17:40-71
Cheng S, Chen S, Liu T, Chang X, Yin Y. Carboxymenthylchitosan as an ecofriendly inhibitor for mild steel in 1 M HCl. Materials Letters. 2007; 61:3276-3280
Cheng S, Chen S, Liu T, Chang X, Yin Y. Carboxymethylchitosan+ Cu 2+ mixture as an inhibitor used for mild steel in 1M HCl. Electrochimica Acta. 2007; 52:5932-5938
Hussein MH, El-Hady MF, Shehata HA, Hegazy MA, Hefni HH. Preparation of some eco-friendly corrosion inhibitors having antibacterial activity from sea food waste. Journal of Surfactants and Detergents. 2013; 16:233-242
Menaka R, Subhashini S. Chitosan Schiff base as effective corrosion inhibitor for mild steel in acid medium. Polymer International. 2017; 66:349-358
Ngo D-H, Vo T-S, Ngo D-N, Kang K-H, Je J-Y, Pham HN-D, Byun H-G, Kim S-K. Biological effects of chitosan and its derivatives. Food Hydrocolloids. 2015; 51:200-216
Vakili M, Rafatullah M, Salamatinia B, Abdullah AZ, Ibrahim MH, Tan KB, Gholami Z, Amouzgar P. Application of chitosan and its derivatives as adsorbents for dye removal from water and wastewater: A review. Carbohydrate Polymers. 2014; 113:115-130
Fekry A, Mohamed RR. Acetyl thiourea chitosan as an eco-friendly inhibitor for mild steel in sulphuric acid medium. Electrochimica Acta. 2010; 55:1933-1939
Muzzarelli RA, Guerrieri M, Goteri G, Muzzarelli C, Armeni T, Ghiselli R, Cornelissen M. The biocompatibility of dibutyryl chitin in the context of wound dressings. Biomaterials. 2005; 26:5844-5854
Li M, Xu J, Li R, Wang D, Li T, Yuan M, Wang J. Simple preparation of aminothiourea-modified chitosan as corrosion inhibitor and heavy metal ion adsorbent. Journal of Colloid and Interface Science. 2014; 417:131-136
Jayakumar R, Nwe N, Tokura S, Tamura H. Sulfated chitin and chitosan as novel biomaterials. International Journal of Biological Macromolecules. 2007; 40:175-181
Balakrishnan B, Mohanty M, Umashankar P, Jayakrishnan A. Evaluation of an in situ forming hydrogel wound dressing based on oxidized alginate and gelatin. Biomaterials. 2005; 26:6335-6342
Abd-El-Nabey B, Gohere Y, Fetouh H, Karam M. Anticorrosive properties of chitosan for the acid corrosion of aluminium. Portugaliae Electrochimica Acta. 2015; 33:231-239
Abboud Y, Abourriche A, Saffaj T, Berrada M, Charrouf M, Bennamara A, Cherqaoui A, Takky D. The inhibition of mild steel corrosion in acidic medium by 2, 2′-bis (benzimidazole). Applied Surface Science. 2006; 252:8178-8184
Bouklah M, Hammouti B, Lagrenee M, Bentiss F. Thermodynamic properties of 2, 5-bis (4-methoxyphenyl)-1, 3, 4-oxadiazole as a corrosion inhibitor for mild steel in normal sulfuric acid medium. Corrosion Science. 2006; 48:2831-2842
Kosari A, Moayed MH, Davoodi A, Parvizi R, Momeni M, Eshghi H, Moradi H. Electrochemical and quantum chemical assessment of two organic compounds from pyridine derivatives as corrosion inhibitors for mild steel in HCl solution under stagnant condition and hydrodynamic flow. Corrosion Science. 2014; 78:138-150
Musa AY, Kadhum AAH, Mohamad AB, Rahoma AAB, Mesmari H. Electrochemical and quantum chemical calculations on 4, 4-dimethyloxazolidine-2-thione as inhibitor for mild steel corrosion in hydrochloric acid. Journal of Molecular Structure. 2010; 969:233-237
Benabdellah M, Tounsi A, Khaled K, Hammouti B. Thermodynamic, chemical and electrochemical investigations of 2-mercapto benzimidazole as corrosion inhibitor for mild steel in hydrochloric acid solutions. Arabian Journal of Chemistry. 2011; 4:17-24
Likhanova NV, Domínguez-Aguilar MA, Olivares-Xometl O, Nava-Entzana N, Arce E, Dorantes H. The effect of ionic liquids with imidazolium and pyridinium cations on the corrosion inhibition of mild steel in acidic environment. Corrosion Science. 2010; 52:2088-2097
Lowmunkhong P, Ungthararak D, Sutthivaiyakit P. Tryptamine as a corrosion inhibitor of mild steel in hydrochloric acid solution. Corrosion Science. 2010; 52:30-36
Larabi L, Harek Y, Benali O, Ghalem S. Hydrazide derivatives as corrosion inhibitors for mild steel in 1 M HCl. Progress in Organic Coatings. 2005; 54:256-262
Ismail KM. Evaluation of cysteine as environmentally friendly corrosion inhibitor for copper in neutral and acidic chloride solutions. Electrochimica Acta. 2007; 52:7811-7819
Umoren SA, Banera MJ, Alonso-Garcia T, Gervasi CA, Mirífico MV. Inhibition of mild steel corrosion in HCl solution using chitosan. Cellulose. 2013; 20:2529-2545
Negm NA, Kandile NG, Badr EA, Mohammed MA. Gravimetric and electrochemical evaluation of environmentally friendly nonionic corrosion inhibitors for carbon steel in 1 M HCl. Corrosion Science. 2012; 65:94-103
Yadav DK, Quraishi MA. Application of some condensed uracils as corrosion inhibitors for mild steel: Gravimetric, electrochemical, surface morphological, UV-visible, and theoretical investigations. Industrial & Engineering Chemistry Research. 2012; 51:14966-14979
Mobin M, Zehra S, Parveen M. L-cysteine as corrosion inhibitor for mild steel in 1 M HCl and synergistic effect of anionic, cationic and non-ionic surfactants. Journal of Molecular Liquids. 2016; 216:598-607
El-Haddad MN. Chitosan as a green inhibitor for copper corrosion in acidic medium. International Journal of Biological Macromolecules. 2013; 55:142-149
Wan K, Feng P, Hou B, Li Y. Enhanced corrosion inhibition properties of carboxymethyl hydroxypropyl chitosan for mild steel in 1.0 M HCl solution. RSC Advances. 2016; 6:77515-77524
Li H, Li H, Liu Y, Huang X. Synthesis of polyamine grafted chitosan copolymer and evaluation of its corrosion inhibition performance. Journal of the Korean Chemical Society. 2015; 59:142-147
Liu Y, Zou C, Yan X, Xiao R, Wang T, Li M. β-Cyclodextrin modified natural chitosan as a green inhibitor for carbon steel in acid solutions. Industrial & Engineering Chemistry Research. 2015; 54:5664-5672
Chauhan DS, Ansari K, Sorour A, Quraishi M, Lgaz H, Salghi R. Thiosemicarbazide and thiocarbohydrazide functionalized chitosan as ecofriendly corrosion inhibitors for carbon steel in hydrochloric acid solution. International Journal of Biological Macromolecules. 2018; 107:1747-1757
Gupta NK, Joshi P, Srivastava V, Quraishi M. Chitosan: A macromolecule as green corrosion inhibitor for mild steel in sulfamic acid useful for sugar industry. International Journal of Biological Macromolecules. 2018; 106:704-711
Pang X, Zhitomirsky I. Electrophoretic deposition of composite hydroxyapatite-chitosan coatings. Materials Characterization. 2007; 58:339-348
Mohamed RR, Fekry A. Antimicrobial and anticorrosive activity of adsorbents based on chitosan Schiff’s base. International Journal of Electrochemical Science. 2011; 6:2488-2508
Ahmed RA, Farghali R, Fekry A. Study for the stability and corrosion inhibition of electrophoretic deposited chitosan on mild steel alloy in acidic medium. International Journal of Electrochemical Science. 2012; 7:7270-7282
Vathsala K, Venkatesha TV, Praveen BM, Nayana KO. Electrochemical generation of Zn-chitosan composite coating on mild steel and its corrosion studies. Engineering. 2010; 2:580
Zheludkevich M, Tedim J, Freire C, Fernandes SC, Kallip S, Lisenkov A, Gandini A, Ferreira M. Self-healing protective coatings with “green” chitosan based pre-layer reservoir of corrosion inhibitor. Journal of Materials Chemistry. 2011; 21:4805-4812
Finšgar M, Uzunalić AP, Stergar J, Gradišnik L, Maver U. Novel chitosan/diclofenac coatings on medical grade stainless steel for hip replacement applications. Scientific Reports. 2016; 6
Lundvall O, Gulppi M, Paez M, Gonzalez E, Zagal J, Pavez J, Thompson G. Copper modified chitosan for protection of AA-2024. Surface and Coatings Technology. 2007; 201:5973-5978
Carneiro J, Tedim J, Fernandes S, Freire C, Gandini A, Ferreira M, Zheludkevich M. Functionalized chitosan-based coatings for active corrosion protection. Surface and Coatings Technology. 2013; 226:51-59
Solomon MM, Gerengi H, Kaya T, Umoren SA. Performance evaluation of a chitosan/silver nanoparticles composite on St37 steel corrosion in a 15% HCl solution. ACS Sustainable Chemistry & Engineering. 2016; 5:809-820
Carneiro J, Tedim J, Fernandes S, Freire C, Silvestre A, Gandini A, Ferreira M, Zheludkevich M. Chitosan-based self-healing protective coatings doped with cerium nitrate for corrosion protection of aluminum alloy 2024. Progress in Organic Coatings. 2012; 75:8-13
Sugama T, Cook M. Poly (itaconic acid)-modified chitosan coatings for mitigating corrosion of aluminum substrates. Progress in Organic Coatings. 2000; 38:79-87